RARE METALS Vol. 25, No. 4, Aug 2006, p . 377
Effects of aging on the microstructures and mechanical properties of extruded AM50 + xCa magnesium alloys WANG Qudong”, PENG Jianguo‘),Sue‘ry Michel”, and Jean-Jacques Blandin2’ 1) National Engineering Research Centre of Light AUoys Net Forming, School of Materials Science and Engineering, Shanghai Jiaotong University,
Shanghai 200030. China 2) Institute National Polytechnique de Grenoble (INPG),(%nie Physique et Mkanique des Matkriaux (GPM2). UMR CNRS 5010, ENS& BP46, 38402 Saint-Martin&Heres Cedex, France (Received 2005-07-26)
Abstract: The effects of aging treatment on the microstructures and mechanical properties of extruded AM50 + xCa alloys (x = 0, 1, 2 wt.%) were studied. The results indicated the secondary phase Mg17A112 precipitated from the saturated a-Mg solid solution while AI2Cachanged slightly when the aging time was increased. The hardness of extruded AM50 + K a alloys increased initially to its peak, and then dropped to reach its original hardness with the increase in aging time. With the increase in aging temperature, the hardness of the AM50 + 2Ca alloy whereas the hardness of AM50 and AM50 + 1Ca alloys derreased in the initial stages of aging treatment and increased in the later stages of aging treabnent The tensile strengths of AM50 and AM50 + 1Ca alloys increased after aging treatment for the precipitation of Mgl7AIl2phase, which increases the resistance against dislocation movement at the grain boundary; with increase in aging temperature, their tensile strengths increased. For AM50 + 2Ca alloy, the tensile strength declined after aging at 150°C and 175”C, while it increased slightly at 200°C. The ductility of AM50 + K a alloys (x = 0 , 1 , 2 wt.%) declined after aging treatment.
Key words: AM50 + K a alloys; aging; extrusion; mechanical properties
[This work was3nancially supported by the International Cooperation Foundation of Shanghai Science and Technology Committee of China (No. 0 2 S W 2 ) and the Regional Council of Rhone-Alpes of France.]
1. Introduction The magnesium alloy, as the lightest structural metal, has been widely used in electronics and aerospace industries [l] owing to its desirable properties. However, magnesium alloys have not been widely used in automobiles so far due to their poor elevated-temperature properties and poor creep resistance. The characteristics of magnesium alloys also restrict their application as a light structural material. The research indicated that wrought magnesium alloys has higher strength, better elongation and other mechanical properties than those of as-cast magnesium alloys ; Ca can increase the elevated-temperature strength and creep resistance of Corresponding author: WANG Qudong
Mg-AI series magnesium alloys [3-4]; aging treatment can improve the microstructure and mechanical properties . However, there are only a few studies on wrought magnesium alloys and few reports about the effect of aging treatment and calcium on wrought magnesium alloys. In this article, the effect of aging treatment on the microstructure and mechanical properties of extruded AM50 + .&a (x = 0, 1,2 wt.%) has been investigated.
2. Experimental The AM50 + xCa (x = 0, 1 , 2 wt.%) magnesium alloys studied here were smelted from commercial AM50 and calcium, and their compositions are
E-mail: wangqudonga sjtu.edu.cn
listed in Table 1. These alloys were melted under SF6 + C02 atmosphere in an electronic resistance furnace and poured into a metal mold. The tensile samples were machined from the as-extruded material. Before extruding, all the specimens were heated to 410°C and held for 30 min. The extruded process is as follows: fmt, extrusion was performed at a mold temperature of 400°C and the extrusion rate was 9:l ($60 mm to $20 mm); second, the as-extruded $20 mm bar was held at 410°C for 30 min, then extrusion was performed at a mold temperature of 315°C and the extrusion rate was 16:l (@20mm to 2 mm x 10 mm). After extrusion, the extruded specimens were solution-treated at 415°C for 20 h and air-cooled. Then the samples were aging-treated at temperatures of 150°C, 175"C, and 200°C for 0.5-24 h. Tensile samples were machined along the extruded direction of the sheets. The microstructure was observed using optical microscopy
RARE METALS, Vol. 25, No. 4, Aug 2006
(LEICA MEF4M). The tensile specimens were tested on the universal test machine (SHIMADZU AGlOOKn A). The hardness was tested on a microhardness tester Oa(-5OO), the experimental load was 19.6 N, and the holding time was 15 s. Table 1. Composition of the studied alloys
AM50 + 1Ca
AM50 + 2Ca
3. Results and discussion 3.1. Microstructures The microstructure of the as-extruded AM50 alloy consists of a-Mg and MgI7All2.As shown in Fig. l(a), some Mg17AlI2surrounds the primary Mg, and the others distributealong the extruded direction.
Fig. 1. Effect of aging treatment on the microstructure of extruded AM50 +x Ca alloys: (a) AM50, T4 (415OC and 24 h); (3)AMSO, T6 (175OC and 1 h); (c) AM50,T6 (175OC and 24 h); (d) AM50 + lCa, T4 (415OC and 24 h); (e) AM50 + 1% T6 (175OC and 1 h); (0AM50 + lCa, T6 (175OC and 24 h); (g) AM50 + 2Ca, T4 (415OC and 24 h); 01) AM50 + 2ca, T6 (175OC and 1 h); (i) AM50 + 2Ca, T6 (175OC and 24 h).
When Ca is added to the AM50 alloy, the number of Mg17A112becomes fewer, the grain size decreases remarkably, and intermetallics A12Ca is found as shown in Figs. l(d) and I&). To show the evolution of microstructure of AM50 + K a alloys in the
course of aging treatment, the samples aging-treated at 175°C are taken as examples. As shown in Figs. l(a-c, d-f), with the increase in aging time, Mg17A112 phase is precipitated from the saturated a-Mg solid solution, whereas AlzCaphase is rather stable, which
Wung Q.D. et ul., Effects of aging on the microstructuresand mechanical properties of.. .
-O-T=lSO"C [email protected]
= 1 75 "C T=200"c
zk 5 8 1
sharply to reach its peak during the continuous precipitation of second phase; for t > 1 h, the hardness decreases because the pattern of precipitation of the second phase changed as the aging treatment continued. As the aging time increased, the unstable second phase transformed from the metastable phase to steady phase, which leads to the decline of hardness. For the AM50 + 2Ca alloy, the hardness decreases with the aging-treatment temperature. For the AM50 + 1Ca and AM50 + 2Ca alloys, the hardness decreases in the initial stages of aging treatment and increases in the later stages of aging treatment. 3.2.2. Tensile properties
i 4 i io Time i h
i 4 i io
Fig.3 shows the effect of aging treatment on the tensile strength of the extruded AM50 + xCa alloys. After aging treatment, Mg17A112phase precipitates from the a-Mg solid solution; however, the A12Ca phase changes slightly. For the AM50 and AM50 + 1Ca alloys, MgI7All2phaseis precipitated in aging treatment, which can resist dislocation movement at the grain boundary and increase the tensile strength of the alloys. For the AM50 + 2Ca alloy, the second phase is mainly A12Ca phase and no Mg17All~phase is precipitated. Therefore, the tensile strength declines after aging at 150°C and 175OC, while it increases slightly at 200°C.
Time i h
150 175 Temperdture / "C
Fig. 3. Effect on aging treatment on the tensile [email protected]
of extruded AM50 + xCa alloys.
t Time i h
Fig. 2. Effect of aging treatment on the hardness of extruded AM50 + xCa magnesium alloys: (a) AM50; (b) AM50 + 1Ca; (c) AM50 + 2Ca.
Fig. 4 shows the effect of aging treatment on the elongation of the extruded AM50 + xCa alloys. After aging treatment, the elongation declines. Besides, with the increase in Ca content, the elongation of AM50 + xCa alloys decreases, for Ca reduces the ductility of the alloys.
RARE METALS, VoL 25, No. 4, Aug 2006
- - AMSDc2Ca
150 175 Temperature I "C
~ i g4.. ~ f f e con t aging treatment on h e elongation of extruded AM50 + xCa alloys.
33. Tensile fracbgraphs Fig. 5 shows tensile fractographs of the extruded AM50 + &a alloys at room temperature after aging treatment at various temperatures. The fractographs display abundant river-like patterns formed by cleavage facets and cleavage steps, which shows that the ductility of alloys is poor and fracture mode is mainly transcrystalline crack. In local areas of the f r a c t o ~ ~ some h s ~ tearing edges can be e n which indicates that quasicleavage cracks exist in local areas.
Fig. 5. Fracture surface SEM of extruded AM50 + xCa alloys after aging treatment: (a) AM50,T6 (15OOCx 20 h); (b)AM!%,T6 (175OCx 20 h); (c) N O , T6 (200°Cx 20 h); (d) AM50 + 1% T6 (1SOOCx 20 h); (e) AM50 + lCa, T6 (175OCx 20 h); (f) AM50 + lCa,T6 (200OCx 24) h); (g) AM50 + 2Ca,T6 (15OOCx 20 h); (h)AM50 + 2Ca,T6 (175OC x 20 h); (i) AM50 + 2Ca,T6 (200OCx 20 h).
Wang Q.D. et ul., Effects of aging on the microstructuresand mechanical properties of.. .
After aging treatment, few tearing edges can be observed. So the ductility of the extruded AM50 + xCa alloys decreases after aging treatment.
while it increases slightly at 200°C. The ductility of all the alloys declines after aging treatment.
References 4. Conclusions (1) With the increase in aging time, MgI7AIl2is precipitated from the saturated solid solution, whereas A2Cais rather stable and changes slightly. (2) In the initial stage of aging treatment, the hardness of the extruded AM50 + xCa alloys increases sharply to reach its peak, then drops to its original hardness in the later stages of aging treatment. For the AM50 + 2Ca alloy, the hardness decreased with the inin aging-treatment temperature.For the AM50 + 1Ca and AM50 + 2Ca alloys, the hardness decreased in the initial stages of aging treatment and increased in the later stages of aging treatment. (3) For the AM50 and AM50 + 1Ca alloys, the tensile strength increases after aging treatment for the precipitation of MgI7Al12phase and the tensile strength increases with the increase in aging temperature. For the AM50 + 2Ca alloy, the tensile strength declines after aging at 150°C and 175"C,
Diem W., Magnesium in different application, Auto Technol.,2001,l: 40. Wang Q.D., Peng J.G, Liu M.P., Chen Y.J, Ding W.J., S d r y M., and Blandin J.J., Microstructure and mechanical extruded properbes of extruded AM50 + xCa magnesium alloys, Mate,: Sci. Forum, 2005, 488-489:119. Liu M.P., Wang Q.D., Zeng X.Q., Lu C., Zhu Y.P., and Ding W.J., Effects of solution heat treatment on the microstructure of Mg-5AI based alloys containing Ca and RE, Rare Met., 2002,21( Suppl.): 54. Wang Q.D., Chen W.Z., Zeng X.Q., Lu Y.Z., Ding W.J., Zhu Y.P., and Xu X.P., Effects of Ca addition on the microstructure and mechanical properties of AZ91 magnesium alloy, J. Mute,: Sci., 2001, 36: 3035. Peng J.G, Wang Q.D., Liu M.P. Chen Y.J. Ding W.J., Suky M., and Blandin J.J., Effect of heat treatment on microstructure and mechanical properties of rolled AM50 + xCa magnesium alloys, Muter: Sci. Forum, 2005,488-489 251.